click-crosslinked injectable hyaluronic acid hydrogel is ... click-crosslinked injectable hyaluronic
Post on 24-Oct-2020
Embed Size (px)
Methods 84 (2015) 60–69
Contents lists available at ScienceDirect
journal homepage: www.elsevier .com/locate /ymeth
Click-crosslinked injectable hyaluronic acid hydrogel is safe and biocompatible in the intrathecal space for ultimate use in regenerative strategies of the injured spinal cord
http://dx.doi.org/10.1016/j.ymeth.2015.03.023 1046-2023/� 2015 Elsevier Inc. All rights reserved.
⇑ Corresponding author at: Department of Chemical Engineering and Applied Chemistry, University of Toronto, 200 College Street, Toronto, Ont. M5S 3E5, Canada.
E-mail address: firstname.lastname@example.org (M.S. Shoichet).
T. Führmann a,b, J. Obermeyer a,b, C.H. Tator c, M.S. Shoichet a,b,⇑ a Department of Chemical Engineering and Applied Chemistry, University of Toronto, 200 College Street, Toronto, Ont. M5S 3E5, Canada b Institute of Biomaterials and Biomedical Engineering, 160 College Street, Room 530, Toronto, Ont. M5S 3E1, Canada c Krembil Neuroscience Centre, Toronto Western Research Institute, and Department of Surgery, University of Toronto, 399 Bathurst Street, Toronto, Ont. M5T 2S8, Canada
a r t i c l e i n f o a b s t r a c t
Article history: Received 14 November 2014 Accepted 26 March 2015 Available online 3 April 2015
Keywords: Hydrogel Spinal cord injury Drug delivery
Traumatic spinal cord injury (SCI) causes damage and degeneration at and around the lesion site resulting in a loss of function. SCI presents a complex regenerative problem due to the multiple aspects of growth inhibition and the heterogeneity in size, shape and extent of injury. Currently, there is no widely accepted treatment strategy available and delivering biomolecules to the central nervous system remains a chal- lenge. With a view towards achieving local release, we designed a hydrogel that can be injected into the intrathecal space. Here we describe the synthesis and characterization of a click-crosslinked hyaluronic acid hydrogel and demonstrate controlled in vitro release of bioactive brain derived neurotrophic factor. Importantly, we demonstrate that this new hydrogel is both biocompatible in the intrathecal space based on immunohistochemistry of the host tissue response and safe based on behavioral analysis of locomotor function.
� 2015 Elsevier Inc. All rights reserved.
Traumatic spinal cord injury (SCI) causes damage and degenera- tion to glia, neurons, and axons at the lesion site, often resulting in permanent loss of function below the site of injury . However, SCI rarely results in complete tissue disruption at the lesion site, and in many cases there is some functional preservation in seg- ments below the injury, indicating survival of functional axons across the lesion . Therefore, minimally invasive treatment strategies, which enhance preservation of nervous tissue at the injury site and promote regeneration of lesioned tissue, are attrac- tive for SCI.
While drug delivery-based treatment strategies hold great pro- mise, prolonged systemic delivery often leads to unwanted side effects, and some of the more promising therapeutic proteins degrade quickly when delivered systemically, often not reaching the spinal cord in efficacious concentrations . Moreover, many therapeutic molecules are unable to cross the blood–spinal cord barrier (BSCB), which limits their accumulation in the spinal cord
after BSCB repair [4,5]. Strategies that deliver therapeutic mole- cules locally avoid some of these obstacles. Two techniques have been used to deliver drugs intrathecally to patients: bolus injec- tion, which is simple, results in the drug being dispersed through- out the central nervous system (CNS) by cerebrospinal fluid (CSF) flow [6,7]; and minipump delivery, where the indwelling catheter may either damage the cord or become obstructed or infected . An alternative strategy, which has significant appeal, is local hydrogel injection, where bioactive molecules are dispersed in the hydrogel, thereby localizing the therapeutic molecule to the spinal cord tissue at the site of injection [9,10]. For the latter, injectable hydrogels should be: (1) injectable through a fine gauge needle for minimally invasive insertion; (2) a gel at the injection site to ensure local delivery; (3) degradable/resorbable to avoid a second procedure for biomaterial removal; and (4) bio-inert, elicit- ing no or minimal toxic or immune response.
Here we describe a hydrogel for intrathecal injection at the site of injury of the spinal cord (see Fig. 1). A small number of injectable hydrogels, categorized as either physical or chemical gels , have been used for spinal cord repair, but only a few have been injected intrathecally [9–11]. Some of these hydrogels have proven to be safe and capable of local delivery of therapeutics to the injured spinal cord [9,11]. These physically-crosslinked gels, while obviat- ing the use of potentially cytotoxic crosslinking agents, are often
Fig. 1. (A) Schematic of the clip compression injury and (B) the hydrogel injection into the intrathecal space on top of the injury. Injection of the hydrogel into the intrathecal space prevents further damage to the spinal cord (compared to direct injection into the tissue).
T. Führmann et al. / Methods 84 (2015) 60–69 61
stable for days to weeks. Chemically crosslinked hydrogels can be tuned to degrade more slowly, thereby providing a route for pro- longed biomolecule delivery to the injured spinal cord . However, chemical gels often require potentially cytotoxic mole- cules for crosslinking, such as coupling agents, catalysts or pho- toinitiators, thereby potentially compromising biocompatibility [12,13]. Crosslinking via disulfide bond formation overcomes some of these problems, yet the polymer structure can be negatively impacted and side reactions with native proteins are likely [13,14]. Click-crosslinked hydrogels provide the advantages of more stable gels without the disadvantages of cytotoxic coupling agents and side products .
Hyaluronic acid (HA) is a major component of the native extra- cellular matrix , but does not form a gel on its own. By reacting HA-furan with poly(ethylene glycol) (PEG) bis-maleimide, a cross- linked hyaluronic acid (xHA) hydrogel is formed based on the Diels–Alder cycloaddition of the HA-furan and PEG-maleimide
[17,18]. Furthermore, HA has been shown to have immunomodu- lating effects and a hydrogel comprised mainly of HA may be ben- eficial on its own for tissue regeneration [9,19–21].
We show that this xHA is safe and biocompatible using an experimental animal model of spinal cord injury, and also allows sustained release of bioactive brain-derived neurotrophic factor (BDNF) in vitro. To test safety and biocompatibility, the xHA hydro- gel was injected intrathecally into both non-injured rats and rats with experimental spinal cord injury using a clinically relevant, moderate clip compression injury model [22,23]. Behavioral and histological analysis demonstrated the safety and biocompatibility of xHA hydrogels, respectively, based on the Basso–Beattie– Bresnahan (BBB) locomotor rating scale , and immunostaining of macrophages, microglia, axons and astrocytes. To assess the util- ity for sustained release of bioactive growth factors, BDNF was encapsulated in poly(lactic-co-glycolic acid) (PLGA) nanoparticles and evaluated for both release, using a BDNF ELISA, and bioactivity
62 T. Führmann et al. / Methods 84 (2015) 60–69
by axonal outgrowth from dorsal root ganglia (DRG). BDNF is com- pelling for SCI repair as it is neuroprotective, enhances motor neu- ron axonal outgrowth and stimulates neuronal differentiation from adult neural stem cells [25–29].
2. Material & methods
2.1. Synthesis and characterization of HA-furan
Furan-modified HA (HA-furan) derivatives were synthesized as described previously . Briefly HA (0.40 g, 1.02 mmol, 2.34 � 105 g/mol, Kikkoman Biochemifa, Tokyo, Japan) was dis- solved in 40 mL of 2-(N-Morpholino)-ethanesulfonic acid (MES) buffer (100 mM, pH 5.5, Fischer Scientific, Ottawa, Canada) to which 4-(4,6-Dimethoxy-1,3,5-triazin-2-yl)-4-methylmorpholin- iumchloride (DMTMM, Sigma–Aldrich, Oakville, Canada) was added in a 2 M ratio (0.56 g, 2.04 mmol, relative to the �COOH groups in HA) and stirred for 10 min. Furfurylamine (Acros Organics, Geel, Belgium) was added dropwise in a 1 M ratio (94.4 ll, 1.02 mmol, relative to the �COOH groups in HA). The reaction was conducted at room temperature for 24 h, dialyzed against 0.1 M sodium chloride in distilled water for 3 days (MW cut-off 12–14 kDa), sterile-filtered through a 0.22 lm PES filter (Nalgene, Rochester, NY, USA), and lyophilized under sterile condi- tions. The degree of substitution (DS) was determined from 1H NMR spectra by comparing the ratio of the areas under the proton peaks at 6.26, 6.46, and 7.65 ppm (furan protons) to the peak at 1.9 ppm (N-acetyl glucosamine protons of HA). 1H NMR spectra were recorded in D2O on a Varian Mercury-400 MHz NMR spec- trometer (Palo Alto, CA) (see Supplemental Fig. 1).
2.2. Synthesis of xHA hydrogels
xHA hydrogels were synthesized by reacting 10 mg of HA-furan (DS 55%, 13.2 lmol of furan) with 7, 10, 13.7 and 20 mg of bis-mal- eimide-poly(ethylene glycol) ((MI)2PEG, 3 kDa, 4.6 lmol of malei- mide, RAPP Polymere GmbH Tübingen, Germany) crosslinker in 960 ll of Dulbecco’s phosphate buffered saline (DPBS, Sigma– Aldrich). We determined 7 mg of (MI)2PEG to be suitable for fur- ther investigations by testing how well the hydrogel is injectable using a 30G needle (see Table 1). The final concentration of HA- furan and (MI)2PEG (furan/MI 1:0.5) in the hydrogels for rheology,